#------------------------------------------------------------------------------
#$Date: 2016-03-22 23:18:03 +0200 (Tue, 22 Mar 2016) $
#$Revision: 179054 $
#$URL: svn://www.crystallography.net/cod/cif/4/30/16/4301648.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4301648
loop_
_publ_author_name
'Monique Tillard'
'David Zitoun'
'Claude Belin'
_publ_contact_author_address
;
Agrégats, Interfaces, Matériaux pour l'Énergie
Institut Charles Gerhardt, UMR 5253 CNRS UM2, CC015,
Université de Montpellier 2, Sciences et Techniques du Languedoc, 
2 Place Eugène Bataillon, 34095 Montpellier Cedex 5 
France
;
_publ_contact_author_email       mtillard@univ-montp2.fr
_publ_contact_author_fax         '33 (0)467 14 33 04  '
_publ_contact_author_name        'Monique TILLARD'
_publ_contact_author_phone       '33 (0)467 14 48 97  '
_publ_section_title
;
Structural Versatility of the ε-SmGax Phase: X-Ray, Electron Diffraction,
and DFT Studies
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              2399
_journal_page_last               2406
_journal_paper_doi               10.1021/ic801379c
_journal_volume                  48
_journal_year                    2009
_chemical_formula_moiety         'Ga2.83 Sm1.06'
_chemical_formula_sum            'Ga2.83 Sm1.06'
_chemical_formula_weight         355.91
_chemical_name_common            'Sm Ga2.67'
_chemical_name_systematic        samarium-gallium
_space_group_IT_number           190
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      190
_symmetry_space_group_name_Hall  'P -6c -2c'
_symmetry_space_group_name_H-M   'P -6 2 c'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            15
_cell_length_a                   12.861(2)
_cell_length_b                   12.861(2)
_cell_length_c                   8.4402(8)
_cell_measurement_reflns_used    19637
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      32.49
_cell_measurement_theta_min      3.03
_cell_volume                     1209.0(3)
_computing_cell_refinement       'CrysAlisRed 171 Oxford Diffraction, 2004'
_computing_data_collection       'CrysAlis 171 Oxford Diffraction, 2004'
_computing_data_reduction        'CrysAlisRed 171 Oxford Diffraction, 2004'
_computing_molecular_graphics    'ORTEP-3 for Windows v.1.075, Farrugia 2002'
_computing_publication_material  'WinGX, Farrugia 1999'
_computing_structure_refinement  'SHELXL-97, Sheldrick, 1997'
_computing_structure_solution    'SHELXS-97, Sheldrick, 1997'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 17
_diffrn_measured_fraction_theta_full 0.962
_diffrn_measured_fraction_theta_max 0.962
_diffrn_measurement_device_type  'Oxford Diffraction Xcalibur CCD'
_diffrn_measurement_method       'omega scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0804
_diffrn_reflns_av_sigmaI/netI    0.0296
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -19
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            19637
_diffrn_reflns_theta_full        32.49
_diffrn_reflns_theta_max         32.49
_diffrn_reflns_theta_min         3.03
_diffrn_standards_decay_%        0
_diffrn_standards_number         4
_exptl_absorpt_coefficient_mu    42.018
_exptl_absorpt_correction_T_max  0.239
_exptl_absorpt_correction_T_min  0.042
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details
;
The reflections were corrected for absorption effects using the SCALE3ABS 
numerical procedure included in the CrysAlis RED software.
;
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    7.332
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       platelet
_exptl_crystal_F_000             2297
_exptl_crystal_size_max          0.14
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.03
_refine_diff_density_max         4.406
_refine_diff_density_min         -3.714
_refine_diff_density_rms         0.585
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.0(9)
_refine_ls_extinction_coef       0.00009(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.131
_refine_ls_matrix_type           full
_refine_ls_number_parameters     61
_refine_ls_number_reflns         1466
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.131
_refine_ls_R_factor_all          0.0884
_refine_ls_R_factor_gt           0.0540
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1075P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1759
_refine_ls_wR_factor_ref         0.1943
_reflns_number_gt                985
_reflns_number_total             1466
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic801379c_si_001_1.cif
_cod_data_source_block           datahex128
_cod_original_cell_volume        1209.1(3)
_cod_database_code               4301648
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'x, y, -z+1/2'
'-y, x-y, -z+1/2'
'-x+y, -x, -z+1/2'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'y, x, z+1/2'
'x-y, -y, z+1/2'
'-x, -x+y, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Sm1 Sm 0.3333 0.6667 0.2500 0.0097(6) Uani 1 6 d S . .
Sm2 Sm 0.32651(13) -0.00053(11) 0.2500 0.0116(5) Uani 1 2 d S . .
Sm3 Sm 0.66299(11) 0.00805(12) 0.2500 0.0106(4) Uani 1 2 d S . .
Sm4 Sm 0.3333 0.6667 0.7500 0.018(2) Uani 0.369(10) 6 d SP . .
Ga4 Ga 0.2245(4) 0.5482(3) 0.7500 0.0188(11) Uani 0.631(10) 2 d SP . .
Sm5 Sm 0.0000 0.0000 0.2500 0.0043(14) Uani 0.572(10) 6 d SP . .
Ga5 Ga 0.1187(6) 0.1134(6) 0.2500 0.028(2) Uani 0.428(10) 2 d SP . .
Ga1 Ga 0.2175(2) 0.77430(19) 0.4820(3) 0.0140(7) Uani 1 1 d . . .
Ga2 Ga 0.44859(19) 0.5589(2) 0.4855(3) 0.0135(7) Uani 1 1 d . . .
Ga3 Ga 0.1114(2) 0.8869(2) 0.5023(2) 0.0248(9) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sm Sm -0.1638 3.4418 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Ga1 Sm1 Ga1 76.37(9) 4 . ?
Ga1 Sm1 Ga1 133.72(3) 4 3_565 ?
Ga1 Sm1 Ga1 85.80(6) . 3_565 ?
Ga1 Sm1 Ga1 85.80(6) 4 5_665 ?
Ga1 Sm1 Ga1 133.72(3) . 5_665 ?
Ga1 Sm1 Ga1 133.72(3) 3_565 5_665 ?
Ga1 Sm1 Ga1 85.80(6) 4 6_565 ?
Ga1 Sm1 Ga1 133.72(3) . 6_565 ?
Ga1 Sm1 Ga1 76.37(9) 3_565 6_565 ?
Ga1 Sm1 Ga1 85.80(6) 5_665 6_565 ?
Ga1 Sm1 Ga1 133.72(3) 4 2_665 ?
Ga1 Sm1 Ga1 85.80(6) . 2_665 ?
Ga1 Sm1 Ga1 85.80(6) 3_565 2_665 ?
Ga1 Sm1 Ga1 76.37(9) 5_665 2_665 ?
Ga1 Sm1 Ga1 133.72(3) 6_565 2_665 ?
Ga1 Sm1 Ga2 94.60(7) 4 2_665 ?
Ga1 Sm1 Ga2 46.20(7) . 2_665 ?
Ga1 Sm1 Ga2 46.05(7) 3_565 2_665 ?
Ga1 Sm1 Ga2 179.52(6) 5_665 2_665 ?
Ga1 Sm1 Ga2 94.49(7) 6_565 2_665 ?
Ga1 Sm1 Ga2 103.16(6) 2_665 2_665 ?
Ga1 Sm1 Ga2 46.05(7) 4 6_565 ?
Ga1 Sm1 Ga2 94.49(7) . 6_565 ?
Ga1 Sm1 Ga2 179.52(6) 3_565 6_565 ?
Ga1 Sm1 Ga2 46.20(7) 5_665 6_565 ?
Ga1 Sm1 Ga2 103.16(6) 6_565 6_565 ?
Ga1 Sm1 Ga2 94.60(7) 2_665 6_565 ?
Ga2 Sm1 Ga2 134.03(3) 2_665 6_565 ?
Ga1 Sm1 Ga2 46.20(7) 4 5_665 ?
Ga1 Sm1 Ga2 94.60(7) . 5_665 ?
Ga1 Sm1 Ga2 94.49(7) 3_565 5_665 ?
Ga1 Sm1 Ga2 103.16(6) 5_665 5_665 ?
Ga1 Sm1 Ga2 46.05(7) 6_565 5_665 ?
Ga1 Sm1 Ga2 179.52(6) 2_665 5_665 ?
Ga2 Sm1 Ga2 77.31(8) 2_665 5_665 ?
Ga2 Sm1 Ga2 85.11(6) 6_565 5_665 ?
Ga1 Sm1 Ga2 94.49(7) 4 3_565 ?
Ga1 Sm1 Ga2 46.05(7) . 3_565 ?
Ga1 Sm1 Ga2 103.16(6) 3_565 3_565 ?
Ga1 Sm1 Ga2 94.60(7) 5_665 3_565 ?
Ga1 Sm1 Ga2 179.52(6) 6_565 3_565 ?
Ga1 Sm1 Ga2 46.20(7) 2_665 3_565 ?
Ga2 Sm1 Ga2 85.11(6) 2_665 3_565 ?
Ga2 Sm1 Ga2 77.31(8) 6_565 3_565 ?
Ga2 Sm1 Ga2 134.03(3) 5_665 3_565 ?
Ga1 Sm1 Ga2 179.52(6) 4 . ?
Ga1 Sm1 Ga2 103.16(6) . . ?
Ga1 Sm1 Ga2 46.20(7) 3_565 . ?
Ga1 Sm1 Ga2 94.49(7) 5_665 . ?
Ga1 Sm1 Ga2 94.60(7) 6_565 . ?
Ga1 Sm1 Ga2 46.05(7) 2_665 . ?
Ga2 Sm1 Ga2 85.11(6) 2_665 . ?
Ga2 Sm1 Ga2 134.03(3) 6_565 . ?
Ga2 Sm1 Ga2 134.03(3) 5_665 . ?
Ga2 Sm1 Ga2 85.11(6) 3_565 . ?
Ga1 Sm1 Ga2 103.16(6) 4 4 ?
Ga1 Sm1 Ga2 179.52(6) . 4 ?
Ga1 Sm1 Ga2 94.60(7) 3_565 4 ?
Ga1 Sm1 Ga2 46.05(7) 5_665 4 ?
Ga1 Sm1 Ga2 46.20(7) 6_565 4 ?
Ga1 Sm1 Ga2 94.49(7) 2_665 4 ?
Ga2 Sm1 Ga2 134.03(3) 2_665 4 ?
Ga2 Sm1 Ga2 85.11(6) 6_565 4 ?
Ga2 Sm1 Ga2 85.11(6) 5_665 4 ?
Ga2 Sm1 Ga2 134.03(3) 3_565 4 ?
Ga2 Sm1 Ga2 77.31(8) . 4 ?
Ga4 Sm2 Ga1 132.88(6) 7_556 4_545 ?
Ga4 Sm2 Ga1 132.88(6) 7_556 1_545 ?
Ga1 Sm2 Ga1 75.96(9) 4_545 1_545 ?
Ga4 Sm2 Ga3 88.09(8) 7_556 8_666 ?
Ga1 Sm2 Ga3 136.59(7) 4_545 8_666 ?
Ga1 Sm2 Ga3 85.32(6) 1_545 8_666 ?
Ga4 Sm2 Ga3 88.09(8) 7_556 11_664 ?
Ga1 Sm2 Ga3 85.32(6) 4_545 11_664 ?
Ga1 Sm2 Ga3 136.59(7) 1_545 11_664 ?
Ga3 Sm2 Ga3 82.06(8) 8_666 11_664 ?
Ga4 Sm2 Ga2 90.02(8) 7_556 5_655 ?
Ga1 Sm2 Ga2 46.01(6) 4_545 5_655 ?
Ga1 Sm2 Ga2 94.10(6) 1_545 5_655 ?
Ga3 Sm2 Ga2 176.81(7) 8_666 5_655 ?
Ga3 Sm2 Ga2 100.44(6) 11_664 5_655 ?
Ga4 Sm2 Ga2 90.02(8) 7_556 2_655 ?
Ga1 Sm2 Ga2 94.10(6) 4_545 2_655 ?
Ga1 Sm2 Ga2 46.01(6) 1_545 2_655 ?
Ga3 Sm2 Ga2 100.44(6) 8_666 2_655 ?
Ga3 Sm2 Ga2 176.81(7) 11_664 2_655 ?
Ga2 Sm2 Ga2 76.98(8) 5_655 2_655 ?
Ga4 Sm2 Ga3 130.75(6) 7_556 4_545 ?
Ga1 Sm2 Ga3 44.93(5) 4_545 4_545 ?
Ga1 Sm2 Ga3 96.29(8) 1_545 4_545 ?
Ga3 Sm2 Ga3 100.56(8) 8_666 4_545 ?
Ga3 Sm2 Ga3 46.46(9) 11_664 4_545 ?
Ga2 Sm2 Ga3 82.62(6) 5_655 4_545 ?
Ga2 Sm2 Ga3 134.30(7) 2_655 4_545 ?
Ga4 Sm2 Ga3 130.75(6) 7_556 1_545 ?
Ga1 Sm2 Ga3 96.29(8) 4_545 1_545 ?
Ga1 Sm2 Ga3 44.93(5) 1_545 1_545 ?
Ga3 Sm2 Ga3 46.46(9) 8_666 1_545 ?
Ga3 Sm2 Ga3 100.56(8) 11_664 1_545 ?
Ga2 Sm2 Ga3 134.30(7) 5_655 1_545 ?
Ga2 Sm2 Ga3 82.62(6) 2_655 1_545 ?
Ga3 Sm2 Ga3 83.24(9) 4_545 1_545 ?
Ga4 Sm2 Ga2 50.32(6) 7_556 9_656 ?
Ga1 Sm2 Ga2 133.64(7) 4_545 9_656 ?
Ga1 Sm2 Ga2 82.60(6) 1_545 9_656 ?
Ga3 Sm2 Ga2 80.41(6) 8_666 9_656 ?
Ga3 Sm2 Ga2 134.99(7) 11_664 9_656 ?
Ga2 Sm2 Ga2 96.41(8) 5_655 9_656 ?
Ga2 Sm2 Ga2 44.22(7) 2_655 9_656 ?
Ga3 Sm2 Ga2 178.48(7) 4_545 9_656 ?
Ga3 Sm2 Ga2 96.65(7) 1_545 9_656 ?
Ga4 Sm2 Ga2 50.32(6) 7_556 12_654 ?
Ga1 Sm2 Ga2 82.60(6) 4_545 12_654 ?
Ga1 Sm2 Ga2 133.64(7) 1_545 12_654 ?
Ga3 Sm2 Ga2 134.99(7) 8_666 12_654 ?
Ga3 Sm2 Ga2 80.41(6) 11_664 12_654 ?
Ga2 Sm2 Ga2 44.22(7) 5_655 12_654 ?
Ga2 Sm2 Ga2 96.41(8) 2_655 12_654 ?
Ga3 Sm2 Ga2 96.65(7) 4_545 12_654 ?
Ga3 Sm2 Ga2 178.48(7) 1_545 12_654 ?
Ga2 Sm2 Ga2 83.42(9) 9_656 12_654 ?
Ga4 Sm2 Ga1 49.02(6) 7_556 8_666 ?
Ga1 Sm2 Ga1 175.76(8) 4_545 8_666 ?
Ga1 Sm2 Ga1 100.09(5) 1_545 8_666 ?
Ga3 Sm2 Ga1 43.48(5) 8_666 8_666 ?
Ga3 Sm2 Ga1 98.70(8) 11_664 8_666 ?
Ga2 Sm2 Ga1 133.74(7) 5_655 8_666 ?
Ga2 Sm2 Ga1 81.95(5) 2_655 8_666 ?
Ga3 Sm2 Ga1 138.02(7) 4_545 8_666 ?
Ga3 Sm2 Ga1 81.73(6) 1_545 8_666 ?
Ga2 Sm2 Ga1 43.37(6) 9_656 8_666 ?
Ga2 Sm2 Ga1 99.32(6) 12_654 8_666 ?
Ga5 Sm3 Ga2 130.92(8) 2_655 5_655 ?
Ga5 Sm3 Ga2 130.92(8) 2_655 2_655 ?
Ga2 Sm3 Ga2 77.57(9) 5_655 2_655 ?
Ga5 Sm3 Ga1 87.99(11) 2_655 6 ?
Ga2 Sm3 Ga1 45.97(6) 5_655 6 ?
Ga2 Sm3 Ga1 94.30(6) 2_655 6 ?
Ga5 Sm3 Ga1 87.99(11) 2_655 3 ?
Ga2 Sm3 Ga1 94.30(6) 5_655 3 ?
Ga2 Sm3 Ga1 45.97(6) 2_655 3 ?
Ga1 Sm3 Ga1 75.85(9) 6 3 ?
Ga5 Sm3 Ga1 88.95(10) 2_655 7_556 ?
Ga2 Sm3 Ga1 138.70(7) 5_655 7_556 ?
Ga2 Sm3 Ga1 83.08(6) 2_655 7_556 ?
Ga1 Sm3 Ga1 173.13(9) 6 7_556 ?
Ga1 Sm3 Ga1 97.90(5) 3 7_556 ?
Ga5 Sm3 Ga1 88.95(10) 2_655 10_554 ?
Ga2 Sm3 Ga1 83.08(6) 5_655 10_554 ?
Ga2 Sm3 Ga1 138.70(7) 2_655 10_554 ?
Ga1 Sm3 Ga1 97.90(5) 6 10_554 ?
Ga1 Sm3 Ga1 173.13(9) 3 10_554 ?
Ga1 Sm3 Ga1 88.19(10) 7_556 10_554 ?
Ga5 Sm3 Ga3 47.45(8) 2_655 7_556 ?
Ga2 Sm3 Ga3 176.16(6) 5_655 7_556 ?
Ga2 Sm3 Ga3 101.14(7) 2_655 7_556 ?
Ga1 Sm3 Ga3 130.95(8) 6 7_556 ?
Ga1 Sm3 Ga3 82.30(6) 3 7_556 ?
Ga1 Sm3 Ga3 44.07(5) 7_556 7_556 ?
Ga1 Sm3 Ga3 100.10(8) 10_554 7_556 ?
Ga5 Sm3 Ga3 47.45(8) 2_655 10_554 ?
Ga2 Sm3 Ga3 101.14(7) 5_655 10_554 ?
Ga2 Sm3 Ga3 176.16(6) 2_655 10_554 ?
Ga1 Sm3 Ga3 82.30(6) 6 10_554 ?
Ga1 Sm3 Ga3 130.95(8) 3 10_554 ?
Ga1 Sm3 Ga3 100.10(8) 7_556 10_554 ?
Ga1 Sm3 Ga3 44.07(5) 10_554 10_554 ?
Ga3 Sm3 Ga3 79.91(9) 7_556 10_554 ?
Ga5 Sm3 Ga2 130.14(7) 2_655 12_654 ?
Ga2 Sm3 Ga2 45.08(7) 5_655 12_654 ?
Ga2 Sm3 Ga2 98.66(7) 2_655 12_654 ?
Ga1 Sm3 Ga2 82.63(6) 6 12_654 ?
Ga1 Sm3 Ga2 135.43(6) 3 12_654 ?
Ga1 Sm3 Ga2 104.02(7) 7_556 12_654 ?
Ga1 Sm3 Ga2 44.81(6) 10_554 12_654 ?
Ga3 Sm3 Ga2 138.73(7) 7_556 12_654 ?
Ga3 Sm3 Ga2 82.73(6) 10_554 12_654 ?
Ga5 Sm3 Ga2 130.14(7) 2_655 9_656 ?
Ga2 Sm3 Ga2 98.66(7) 5_655 9_656 ?
Ga2 Sm3 Ga2 45.08(7) 2_655 9_656 ?
Ga1 Sm3 Ga2 135.43(6) 6 9_656 ?
Ga1 Sm3 Ga2 82.63(6) 3 9_656 ?
Ga1 Sm3 Ga2 44.81(6) 7_556 9_656 ?
Ga1 Sm3 Ga2 104.02(7) 10_554 9_656 ?
Ga3 Sm3 Ga2 82.73(6) 7_556 9_656 ?
Ga3 Sm3 Ga2 138.73(7) 10_554 9_656 ?
Ga2 Sm3 Ga2 86.28(8) 12_654 9_656 ?
Ga5 Sm3 Ga3 48.26(8) 2_655 3 ?
Ga2 Sm3 Ga3 132.02(7) 5_655 3 ?
Ga2 Sm3 Ga3 82.69(6) 2_655 3 ?
Ga1 Sm3 Ga3 93.43(8) 6 3 ?
Ga1 Sm3 Ga3 43.79(5) 3 3 ?
Ga1 Sm3 Ga3 79.95(6) 7_556 3 ?
Ga1 Sm3 Ga3 135.28(7) 10_554 3 ?
Ga3 Sm3 Ga3 44.14(8) 7_556 3 ?
Ga3 Sm3 Ga3 95.69(8) 10_554 3 ?
Ga2 Sm3 Ga3 175.91(6) 12_654 3 ?
Ga2 Sm3 Ga3 97.34(6) 9_656 3 ?
Ga4 Sm4 Ga4 120.000(1) 3_565 . ?
Ga4 Sm4 Ga4 120.000(1) 3_565 2_665 ?
Ga4 Sm4 Ga4 120.0 . 2_665 ?
Ga4 Sm4 Ga2 51.44(10) 3_565 5_666 ?
Ga4 Sm4 Ga2 131.54(9) . 5_666 ?
Ga4 Sm4 Ga2 87.72(13) 2_665 5_666 ?
Ga4 Sm4 Ga2 87.72(13) 3_565 3_565 ?
Ga4 Sm4 Ga2 51.44(10) . 3_565 ?
Ga4 Sm4 Ga2 131.54(9) 2_665 3_565 ?
Ga2 Sm4 Ga2 136.33(3) 5_666 3_565 ?
Ga4 Sm4 Ga2 51.44(10) 3_565 2_665 ?
Ga4 Sm4 Ga2 131.54(9) . 2_665 ?
Ga4 Sm4 Ga2 87.72(13) 2_665 2_665 ?
Ga2 Sm4 Ga2 83.89(7) 5_666 2_665 ?
Ga2 Sm4 Ga2 80.20(5) 3_565 2_665 ?
Ga4 Sm4 Ga2 87.72(13) 3_565 6_566 ?
Ga4 Sm4 Ga2 51.44(9) . 6_566 ?
Ga4 Sm4 Ga2 131.54(9) 2_665 6_566 ?
Ga2 Sm4 Ga2 80.20(5) 5_666 6_566 ?
Ga2 Sm4 Ga2 83.89(7) 3_565 6_566 ?
Ga2 Sm4 Ga2 136.33(3) 2_665 6_566 ?
Ga4 Sm4 Ga2 131.54(9) 3_565 . ?
Ga4 Sm4 Ga2 87.72(13) . . ?
Ga4 Sm4 Ga2 51.44(9) 2_665 . ?
Ga2 Sm4 Ga2 136.33(3) 5_666 . ?
Ga2 Sm4 Ga2 80.20(5) 3_565 . ?
Ga2 Sm4 Ga2 80.20(5) 2_665 . ?
Ga2 Sm4 Ga2 136.33(3) 6_566 . ?
Ga4 Sm4 Ga2 131.54(9) 3_565 4_556 ?
Ga4 Sm4 Ga2 87.72(13) . 4_556 ?
Ga4 Sm4 Ga2 51.44(9) 2_665 4_556 ?
Ga2 Sm4 Ga2 80.20(5) 5_666 4_556 ?
Ga2 Sm4 Ga2 136.33(3) 3_565 4_556 ?
Ga2 Sm4 Ga2 136.33(3) 2_665 4_556 ?
Ga2 Sm4 Ga2 80.20(5) 6_566 4_556 ?
Ga2 Sm4 Ga2 83.89(7) . 4_556 ?
Ga4 Sm4 Ga1 48.75(9) 3_565 . ?
Ga4 Sm4 Ga1 92.19(13) . . ?
Ga4 Sm4 Ga1 128.39(9) 2_665 . ?
Ga2 Sm4 Ga1 100.08(6) 5_666 . ?
Ga2 Sm4 Ga1 43.48(7) 3_565 . ?
Ga2 Sm4 Ga1 43.63(7) 2_665 . ?
Ga2 Sm4 Ga1 99.98(6) 6_566 . ?
Ga2 Sm4 Ga1 95.81(5) . . ?
Ga2 Sm4 Ga1 179.68(5) 4_556 . ?
Ga4 Sm4 Ga1 48.75(9) 3_565 4_556 ?
Ga4 Sm4 Ga1 92.19(13) . 4_556 ?
Ga4 Sm4 Ga1 128.39(9) 2_665 4_556 ?
Ga2 Sm4 Ga1 43.63(7) 5_666 4_556 ?
Ga2 Sm4 Ga1 99.98(6) 3_565 4_556 ?
Ga2 Sm4 Ga1 100.08(6) 2_665 4_556 ?
Ga2 Sm4 Ga1 43.48(7) 6_566 4_556 ?
Ga2 Sm4 Ga1 179.68(5) . 4_556 ?
Ga2 Sm4 Ga1 95.81(5) 4_556 4_556 ?
Ga1 Sm4 Ga1 84.50(7) . 4_556 ?
Ga4 Sm4 Ga1 92.19(13) 3_565 6_566 ?
Ga4 Sm4 Ga1 128.39(9) . 6_566 ?
Ga4 Sm4 Ga1 48.75(8) 2_665 6_566 ?
Ga2 Sm4 Ga1 43.48(7) 5_666 6_566 ?
Ga2 Sm4 Ga1 179.68(6) 3_565 6_566 ?
Ga2 Sm4 Ga1 99.98(6) 2_665 6_566 ?
Ga2 Sm4 Ga1 95.81(5) 6_566 6_566 ?
Ga2 Sm4 Ga1 100.08(6) . 6_566 ?
Ga2 Sm4 Ga1 43.63(7) 4_556 6_566 ?
Ga1 Sm4 Ga1 136.56(3) . 6_566 ?
Ga1 Sm4 Ga1 79.74(6) 4_556 6_566 ?
Sm4 Ga4 Ga4 30.0 . 2_665 ?
Sm4 Ga4 Ga4 30.0 . 3_565 ?
Ga4 Ga4 Ga4 60.000(1) 2_665 3_565 ?
Sm4 Ga4 Ga1 106.56(13) . 2_665 ?
Ga4 Ga4 Ga1 91.86(16) 2_665 2_665 ?
Ga4 Ga4 Ga1 117.47(8) 3_565 2_665 ?
Sm4 Ga4 Ga1 106.56(13) . 5_666 ?
Ga4 Ga4 Ga1 91.86(16) 2_665 5_666 ?
Ga4 Ga4 Ga1 117.47(8) 3_565 5_666 ?
Ga1 Ga4 Ga1 118.00(17) 2_665 5_666 ?
Sm4 Ga4 Ga2 103.28(13) . 3_565 ?
Ga4 Ga4 Ga2 116.84(8) 2_665 3_565 ?
Ga4 Ga4 Ga2 86.92(15) 3_565 3_565 ?
Ga1 Ga4 Ga2 55.81(9) 2_665 3_565 ?
Ga1 Ga4 Ga2 149.80(17) 5_666 3_565 ?
Sm4 Ga4 Ga2 103.28(13) . 6_566 ?
Ga4 Ga4 Ga2 116.84(8) 2_665 6_566 ?
Ga4 Ga4 Ga2 86.92(15) 3_565 6_566 ?
Ga1 Ga4 Ga2 149.80(17) 2_665 6_566 ?
Ga1 Ga4 Ga2 55.81(9) 5_666 6_566 ?
Ga2 Ga4 Ga2 112.59(19) 3_565 6_566 ?
Sm4 Ga4 Sm2 175.1(2) . 7_556 ?
Ga4 Ga4 Sm2 154.9(2) 2_665 7_556 ?
Ga4 Ga4 Sm2 145.1(2) 3_565 7_556 ?
Ga1 Ga4 Sm2 75.68(9) 2_665 7_556 ?
Ga1 Ga4 Sm2 75.68(9) 5_666 7_556 ?
Ga2 Ga4 Sm2 74.21(10) 3_565 7_556 ?
Ga2 Ga4 Sm2 74.21(10) 6_566 7_556 ?
Ga5 Sm5 Ga5 120.0 . 3 ?
Ga5 Sm5 Ga5 120.0 . 2 ?
Ga5 Sm5 Ga5 120.000(1) 3 2 ?
Ga5 Sm5 Ga3 130.32(14) . 12_544 ?
Ga5 Sm5 Ga3 47.11(13) 3 12_544 ?
Ga5 Sm5 Ga3 91.9(2) 2 12_544 ?
Ga5 Sm5 Ga3 47.11(13) . 8_666 ?
Ga5 Sm5 Ga3 91.9(2) 3 8_666 ?
Ga5 Sm5 Ga3 130.32(14) 2 8_666 ?
Ga3 Sm5 Ga3 134.88(3) 12_544 8_666 ?
Ga5 Sm5 Ga3 91.9(2) . 10_454 ?
Ga5 Sm5 Ga3 130.32(14) 3 10_454 ?
Ga5 Sm5 Ga3 47.11(13) 2 10_454 ?
Ga3 Sm5 Ga3 83.28(6) 12_544 10_454 ?
Ga3 Sm5 Ga3 134.88(3) 8_666 10_454 ?
Ga5 Sm5 Ga3 91.9(2) . 7_456 ?
Ga5 Sm5 Ga3 130.32(14) 3 7_456 ?
Ga5 Sm5 Ga3 47.11(13) 2 7_456 ?
Ga3 Sm5 Ga3 134.88(3) 12_544 7_456 ?
Ga3 Sm5 Ga3 83.28(6) 8_666 7_456 ?
Ga3 Sm5 Ga3 79.79(8) 10_454 7_456 ?
Ga5 Sm5 Ga3 47.11(13) . 11_664 ?
Ga5 Sm5 Ga3 91.9(2) 3 11_664 ?
Ga5 Sm5 Ga3 130.32(14) 2 11_664 ?
Ga3 Sm5 Ga3 83.28(6) 12_544 11_664 ?
Ga3 Sm5 Ga3 79.79(8) 8_666 11_664 ?
Ga3 Sm5 Ga3 83.28(6) 10_454 11_664 ?
Ga3 Sm5 Ga3 134.88(3) 7_456 11_664 ?
Ga5 Sm5 Ga3 130.32(14) . 9_546 ?
Ga5 Sm5 Ga3 47.11(13) 3 9_546 ?
Ga5 Sm5 Ga3 91.9(2) 2 9_546 ?
Ga3 Sm5 Ga3 79.79(8) 12_544 9_546 ?
Ga3 Sm5 Ga3 83.28(6) 8_666 9_546 ?
Ga3 Sm5 Ga3 134.88(3) 10_454 9_546 ?
Ga3 Sm5 Ga3 83.28(6) 7_456 9_546 ?
Ga3 Sm5 Ga3 134.88(3) 11_664 9_546 ?
Ga5 Sm5 Ga3 49.77(14) . 2_665 ?
Ga5 Sm5 Ga3 132.25(13) 3 2_665 ?
Ga5 Sm5 Ga3 88.48(19) 2 2_665 ?
Ga3 Sm5 Ga3 179.36(7) 12_544 2_665 ?
Ga3 Sm5 Ga3 44.58(8) 8_666 2_665 ?
Ga3 Sm5 Ga3 97.36(7) 10_454 2_665 ?
Ga3 Sm5 Ga3 45.30(8) 7_456 2_665 ?
Ga3 Sm5 Ga3 96.84(7) 11_664 2_665 ?
Ga3 Sm5 Ga3 99.70(5) 9_546 2_665 ?
Ga5 Sm5 Ga3 132.25(13) . 6_455 ?
Ga5 Sm5 Ga3 88.48(19) 3 6_455 ?
Ga5 Sm5 Ga3 49.77(14) 2 6_455 ?
Ga3 Sm5 Ga3 45.30(8) 12_544 6_455 ?
Ga3 Sm5 Ga3 179.36(7) 8_666 6_455 ?
Ga3 Sm5 Ga3 44.58(8) 10_454 6_455 ?
Ga3 Sm5 Ga3 96.84(7) 7_456 6_455 ?
Ga3 Sm5 Ga3 99.70(5) 11_664 6_455 ?
Ga3 Sm5 Ga3 97.36(7) 9_546 6_455 ?
Ga3 Sm5 Ga3 135.24(3) 2_665 6_455 ?
Ga5 Sm5 Ga3 88.48(19) . 1_545 ?
Ga5 Sm5 Ga3 49.77(14) 3 1_545 ?
Ga5 Sm5 Ga3 132.25(13) 2 1_545 ?
Ga3 Sm5 Ga3 96.84(7) 12_544 1_545 ?
Ga3 Sm5 Ga3 45.30(8) 8_666 1_545 ?
Ga3 Sm5 Ga3 179.36(6) 10_454 1_545 ?
Ga3 Sm5 Ga3 99.70(5) 7_456 1_545 ?
Ga3 Sm5 Ga3 97.36(7) 11_664 1_545 ?
Ga3 Sm5 Ga3 44.58(8) 9_546 1_545 ?
Ga3 Sm5 Ga3 82.52(6) 2_665 1_545 ?
Ga3 Sm5 Ga3 135.24(3) 6_455 1_545 ?
Sm5 Ga5 Ga3 106.9(2) . 8_666 ?
Sm5 Ga5 Ga3 106.9(2) . 11_664 ?
Ga3 Ga5 Ga3 113.8(3) 8_666 11_664 ?
Sm5 Ga5 Ga3 104.1(2) . 2_665 ?
Ga3 Ga5 Ga3 58.45(11) 8_666 2_665 ?
Ga3 Ga5 Ga3 148.9(3) 11_664 2_665 ?
Sm5 Ga5 Ga3 104.1(2) . 5_665 ?
Ga3 Ga5 Ga3 148.9(3) 8_666 5_665 ?
Ga3 Ga5 Ga3 58.45(11) 11_664 5_665 ?
Ga3 Ga5 Ga3 110.9(3) 2_665 5_665 ?
Sm5 Ga5 Ga5 30.0 . 3 ?
Ga3 Ga5 Ga5 91.2(3) 8_666 3 ?
Ga3 Ga5 Ga5 91.2(3) 11_664 3 ?
Ga3 Ga5 Ga5 117.82(15) 2_665 3 ?
Ga3 Ga5 Ga5 117.82(15) 5_665 3 ?
Sm5 Ga5 Ga5 30.0 . 2 ?
Ga3 Ga5 Ga5 118.88(15) 8_666 2 ?
Ga3 Ga5 Ga5 118.88(15) 11_664 2 ?
Ga3 Ga5 Ga5 87.4(3) 2_665 2 ?
Ga3 Ga5 Ga5 87.4(3) 5_665 2 ?
Ga5 Ga5 Ga5 60.0 3 2 ?
Sm5 Ga5 Sm3 178.4(4) . 3_665 ?
Ga3 Ga5 Sm3 73.90(18) 8_666 3_665 ?
Ga3 Ga5 Sm3 73.90(18) 11_664 3_665 ?
Ga3 Ga5 Sm3 75.09(18) 2_665 3_665 ?
Ga3 Ga5 Sm3 75.09(18) 5_665 3_665 ?
Ga5 Ga5 Sm3 151.6(4) 3 3_665 ?
Ga5 Ga5 Sm3 148.4(4) 2 3_665 ?
Ga3 Ga1 Ga2 122.11(8) . 3_565 ?
Ga3 Ga1 Ga2 117.83(8) . 2_665 ?
Ga2 Ga1 Ga2 119.77(12) 3_565 2_665 ?
Ga3 Ga1 Ga4 112.20(12) . 3_565 ?
Ga2 Ga1 Ga4 89.07(12) 3_565 3_565 ?
Ga2 Ga1 Ga4 63.02(12) 2_665 3_565 ?
Ga3 Ga1 Sm1 145.76(11) . . ?
Ga2 Ga1 Sm1 67.27(7) 3_565 . ?
Ga2 Ga1 Sm1 67.19(7) 2_665 . ?
Ga4 Ga1 Sm1 100.20(9) 3_565 . ?
Ga3 Ga1 Sm2 68.04(6) . 1_565 ?
Ga2 Ga1 Sm2 142.69(11) 3_565 1_565 ?
Ga2 Ga1 Sm2 67.23(6) 2_665 1_565 ?
Ga4 Ga1 Sm2 122.06(12) 3_565 1_565 ?
Sm1 Ga1 Sm2 85.85(6) . 1_565 ?
Ga3 Ga1 Sm3 71.63(7) . 2 ?
Ga2 Ga1 Sm3 66.73(7) 3_565 2 ?
Ga2 Ga1 Sm3 142.73(10) 2_665 2 ?
Ga4 Ga1 Sm3 150.90(13) 3_565 2 ?
Sm1 Ga1 Sm3 85.60(6) . 2 ?
Sm2 Ga1 Sm3 86.62(7) 1_565 2 ?
Ga3 Ga1 Sm3 68.09(6) . 7_556 ?
Ga2 Ga1 Sm3 67.92(7) 3_565 7_556 ?
Ga2 Ga1 Sm3 135.23(11) 2_665 7_556 ?
Ga4 Ga1 Sm3 73.67(10) 3_565 7_556 ?
Sm1 Ga1 Sm3 134.83(8) . 7_556 ?
Sm2 Ga1 Sm3 136.07(7) 1_565 7_556 ?
Sm3 Ga1 Sm3 82.02(5) 2 7_556 ?
Ga3 Ga1 Sm4 133.70(10) . . ?
Ga2 Ga1 Sm4 67.76(7) 3_565 . ?
Ga2 Ga1 Sm4 67.69(8) 2_665 . ?
Ga4 Ga1 Sm4 24.69(8) 3_565 . ?
Sm1 Ga1 Sm4 80.44(4) . . ?
Sm2 Ga1 Sm4 134.75(7) 1_565 . ?
Sm3 Ga1 Sm4 134.33(8) 2 . ?
Sm3 Ga1 Sm4 77.93(6) 7_556 . ?
Ga3 Ga1 Sm2 63.87(7) . 8_566 ?
Ga2 Ga1 Sm2 137.43(10) 3_565 8_566 ?
Ga2 Ga1 Sm2 67.66(6) 2_665 8_566 ?
Ga4 Ga1 Sm2 55.29(9) 3_565 8_566 ?
Sm1 Ga1 Sm2 134.74(7) . 8_566 ?
Sm2 Ga1 Sm2 79.89(5) 1_565 8_566 ?
Sm3 Ga1 Sm2 135.40(7) 2 8_566 ?
Sm3 Ga1 Sm2 79.10(6) 7_556 8_566 ?
Sm4 Ga1 Sm2 79.91(6) . 8_566 ?
Ga2 Ga2 Ga1 118.65(6) 7_556 2_665 ?
Ga2 Ga2 Ga1 120.96(6) 7_556 3_565 ?
Ga1 Ga2 Ga1 120.20(12) 2_665 3_565 ?
Ga2 Ga2 Ga4 112.88(14) 7_556 2_665 ?
Ga1 Ga2 Ga4 92.02(12) 2_665 2_665 ?
Ga1 Ga2 Ga4 61.17(12) 3_565 2_665 ?
Ga2 Ga2 Sm3 69.44(7) 7_556 3_665 ?
Ga1 Ga2 Sm3 67.30(6) 2_665 3_665 ?
Ga1 Ga2 Sm3 140.54(10) 3_565 3_665 ?
Ga4 Ga2 Sm3 155.30(12) 2_665 3_665 ?
Ga2 Ga2 Sm1 147.03(14) 7_556 . ?
Ga1 Ga2 Sm1 66.68(7) 2_665 . ?
Ga1 Ga2 Sm1 66.61(8) 3_565 . ?
Ga4 Ga2 Sm1 98.86(10) 2_665 . ?
Sm3 Ga2 Sm1 85.59(5) 3_665 . ?
Ga2 Ga2 Sm2 71.39(7) 7_556 3_665 ?
Ga1 Ga2 Sm2 140.84(9) 2_665 3_665 ?
Ga1 Ga2 Sm2 66.77(7) 3_565 3_665 ?
Ga4 Ga2 Sm2 120.13(12) 2_665 3_665 ?
Sm3 Ga2 Sm2 84.33(6) 3_665 3_665 ?
Sm1 Ga2 Sm2 85.44(6) . 3_665 ?
Ga2 Ga2 Sm3 65.48(7) 7_556 9_666 ?
Ga1 Ga2 Sm3 67.27(7) 2_665 9_666 ?
Ga1 Ga2 Sm3 137.46(9) 3_565 9_666 ?
Ga4 Ga2 Sm3 77.38(10) 2_665 9_666 ?
Sm3 Ga2 Sm3 81.99(5) 3_665 9_666 ?
Sm1 Ga2 Sm3 133.61(7) . 9_666 ?
Sm2 Ga2 Sm3 136.85(7) 3_665 9_666 ?
Ga2 Ga2 Sm4 132.34(13) 7_556 . ?
Ga1 Ga2 Sm4 68.76(8) 2_665 . ?
Ga1 Ga2 Sm4 68.68(8) 3_565 . ?
Ga4 Ga2 Sm4 25.28(8) 2_665 . ?
Sm3 Ga2 Sm4 135.90(7) 3_665 . ?
Sm1 Ga2 Sm4 80.60(5) . . ?
Sm2 Ga2 Sm4 135.29(8) 3_665 . ?
Sm3 Ga2 Sm4 78.06(6) 9_666 . ?
Ga2 Ga2 Sm2 64.39(7) 7_556 9_666 ?
Ga1 Ga2 Sm2 138.95(10) 2_665 9_666 ?
Ga1 Ga2 Sm2 68.97(6) 3_565 9_666 ?
Ga4 Ga2 Sm2 55.47(9) 2_665 9_666 ?
Sm3 Ga2 Sm2 133.82(7) 3_665 9_666 ?
Sm1 Ga2 Sm2 135.45(7) . 9_666 ?
Sm2 Ga2 Sm2 80.20(6) 3_665 9_666 ?
Sm3 Ga2 Sm2 80.39(6) 9_666 9_666 ?
Sm4 Ga2 Sm2 80.69(5) . 9_666 ?
Ga1 Ga3 Ga3 118.86(4) . 9_556 ?
Ga1 Ga3 Ga5 121.68(18) . 8_566 ?
Ga3 Ga3 Ga5 62.56(16) 9_556 8_566 ?
Ga1 Ga3 Ga3 120.83(4) . 8_676 ?
Ga3 Ga3 Ga3 119.977(5) 9_556 8_676 ?
Ga5 Ga3 Ga3 90.8(2) 8_566 8_676 ?
Ga1 Ga3 Ga5 114.51(17) . 3_565 ?
Ga3 Ga3 Ga5 58.98(15) 9_556 3_565 ?
Ga5 Ga3 Ga5 112.34(16) 8_566 3_565 ?
Ga3 Ga3 Ga5 90.65(18) 8_676 3_565 ?
Ga1 Ga3 Sm2 72.65(8) . 8_566 ?
Ga3 Ga3 Sm2 139.82(12) 9_556 8_566 ?
Ga5 Ga3 Sm2 78.51(14) 8_566 8_566 ?
Ga3 Ga3 Sm2 67.20(8) 8_676 8_566 ?
Ga5 Ga3 Sm2 155.98(18) 3_565 8_566 ?
Ga1 Ga3 Sm2 67.03(6) . 1_565 ?
Ga3 Ga3 Sm2 137.47(13) 9_556 1_565 ?
Ga5 Ga3 Sm2 154.79(19) 8_566 1_565 ?
Ga3 Ga3 Sm2 66.34(7) 8_676 1_565 ?
Ga5 Ga3 Sm2 79.82(14) 3_565 1_565 ?
Sm2 Ga3 Sm2 82.65(6) 8_566 1_565 ?
Ga1 Ga3 Sm3 67.84(7) . 7_556 ?
Ga3 Ga3 Sm3 69.90(7) 9_556 7_556 ?
Ga5 Ga3 Sm3 58.65(17) 8_566 7_556 ?
Ga3 Ga3 Sm3 140.85(13) 8_676 7_556 ?
Ga5 Ga3 Sm3 121.99(17) 3_565 7_556 ?
Sm2 Ga3 Sm3 82.02(5) 8_566 7_556 ?
Sm2 Ga3 Sm3 134.80(8) 1_565 7_556 ?
Ga1 Ga3 Sm5 144.11(10) . 7_566 ?
Ga3 Ga3 Sm5 68.24(7) 9_556 7_566 ?
Ga5 Ga3 Sm5 26.00(16) 8_566 7_566 ?
Ga3 Ga3 Sm5 67.87(7) 8_676 7_566 ?
Ga5 Ga3 Sm5 99.31(16) 3_565 7_566 ?
Sm2 Ga3 Sm5 81.38(6) 8_566 7_566 ?
Sm2 Ga3 Sm5 134.18(8) 1_565 7_566 ?
Sm3 Ga3 Sm5 84.64(5) 7_556 7_566 ?
Ga1 Ga3 Sm5 135.58(9) . 1_565 ?
Ga3 Ga3 Sm5 67.18(7) 9_556 1_565 ?
Ga5 Ga3 Sm5 100.60(16) 8_566 1_565 ?
Ga3 Ga3 Sm5 66.83(7) 8_676 1_565 ?
Ga5 Ga3 Sm5 26.17(16) 3_565 1_565 ?
Sm2 Ga3 Sm5 134.00(8) 8_566 1_565 ?
Sm2 Ga3 Sm5 80.70(5) 1_565 1_565 ?
Sm3 Ga3 Sm5 137.08(8) 7_556 1_565 ?
Sm5 Ga3 Sm5 80.30(5) 7_566 1_565 ?
Ga1 Ga3 Sm3 64.59(7) . 2 ?
Ga3 Ga3 Sm3 65.97(7) 9_556 2 ?
Ga5 Ga3 Sm3 121.63(18) 8_566 2 ?
Ga3 Ga3 Sm3 139.63(12) 8_676 2 ?
Ga5 Ga3 Sm3 56.65(16) 3_565 2 ?
Sm2 Ga3 Sm3 137.13(9) 8_566 2 ?
Sm2 Ga3 Sm3 83.58(5) 1_565 2 ?
Sm3 Ga3 Sm3 79.51(7) 7_556 2 ?
Sm5 Ga3 Sm3 134.20(8) 7_566 2 ?
Sm5 Ga3 Sm3 82.81(5) 1_565 2 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Sm1 Ga1 3.168(2) 4 ?
Sm1 Ga1 3.168(2) . ?
Sm1 Ga1 3.168(2) 3_565 ?
Sm1 Ga1 3.168(2) 5_665 ?
Sm1 Ga1 3.168(2) 6_565 ?
Sm1 Ga1 3.168(2) 2_665 ?
Sm1 Ga2 3.182(2) 2_665 ?
Sm1 Ga2 3.182(2) 6_565 ?
Sm1 Ga2 3.182(2) 5_665 ?
Sm1 Ga2 3.182(2) 3_565 ?
Sm1 Ga2 3.182(2) . ?
Sm1 Ga2 3.182(2) 4 ?
Sm2 Ga4 2.873(4) 7_556 ?
Sm2 Ga1 3.182(2) 4_545 ?
Sm2 Ga1 3.182(2) 1_545 ?
Sm2 Ga3 3.185(2) 8_666 ?
Sm2 Ga3 3.185(2) 11_664 ?
Sm2 Ga2 3.193(2) 5_655 ?
Sm2 Ga2 3.193(2) 2_655 ?
Sm2 Ga3 3.206(2) 4_545 ?
Sm2 Ga3 3.206(2) 1_545 ?
Sm2 Ga2 3.356(2) 9_656 ?
Sm2 Ga2 3.356(2) 12_654 ?
Sm2 Ga1 3.386(3) 8_666 ?
Sm3 Ga5 2.894(7) 2_655 ?
Sm3 Ga2 3.173(2) 5_655 ?
Sm3 Ga2 3.173(2) 2_655 ?
Sm3 Ga1 3.186(3) 6 ?
Sm3 Ga1 3.186(3) 3 ?
Sm3 Ga1 3.250(2) 7_556 ?
Sm3 Ga1 3.250(2) 10_554 ?
Sm3 Ga3 3.256(3) 7_556 ?
Sm3 Ga3 3.256(3) 10_554 ?
Sm3 Ga2 3.265(2) 12_654 ?
Sm3 Ga2 3.265(2) 9_656 ?
Sm3 Ga3 3.348(3) 3 ?
Sm4 Ga4 1.466(4) 3_565 ?
Sm4 Ga4 1.466(4) . ?
Sm4 Ga4 1.466(4) 2_665 ?
Sm4 Ga2 3.340(2) 5_666 ?
Sm4 Ga2 3.340(2) 3_565 ?
Sm4 Ga2 3.340(2) 2_665 ?
Sm4 Ga2 3.340(2) 6_566 ?
Sm4 Ga2 3.340(2) . ?
Sm4 Ga2 3.340(2) 4_556 ?
Sm4 Ga1 3.364(2) . ?
Sm4 Ga1 3.364(2) 4_556 ?
Sm4 Ga1 3.364(2) 6_566 ?
Ga4 Ga4 2.539(6) 2_665 ?
Ga4 Ga4 2.539(6) 3_565 ?
Ga4 Ga1 2.638(3) 2_665 ?
Ga4 Ga1 2.638(3) 5_666 ?
Ga4 Ga2 2.684(3) 3_565 ?
Ga4 Ga2 2.684(3) 6_566 ?
Ga4 Sm2 2.873(4) 7_556 ?
Sm5 Ga5 1.493(7) . ?
Sm5 Ga5 1.493(7) 3 ?
Sm5 Ga5 1.493(7) 2 ?
Sm5 Ga3 3.260(2) 12_544 ?
Sm5 Ga3 3.260(2) 8_666 ?
Sm5 Ga3 3.260(2) 10_454 ?
Sm5 Ga3 3.260(2) 7_456 ?
Sm5 Ga3 3.260(2) 11_664 ?
Sm5 Ga3 3.260(2) 9_546 ?
Sm5 Ga3 3.285(2) 2_665 ?
Sm5 Ga3 3.285(2) 6_455 ?
Sm5 Ga3 3.285(2) 1_545 ?
Ga5 Ga3 2.496(4) 8_666 ?
Ga5 Ga3 2.496(4) 11_664 ?
Ga5 Ga3 2.585(4) 2_665 ?
Ga5 Ga3 2.585(4) 5_665 ?
Ga5 Ga5 2.587(12) 3 ?
Ga5 Ga5 2.587(12) 2 ?
Ga5 Sm3 2.894(7) 3_665 ?
Ga1 Ga3 2.441(2) . ?
Ga1 Ga2 2.483(4) 3_565 ?
Ga1 Ga2 2.491(4) 2_665 ?
Ga1 Ga4 2.638(3) 3_565 ?
Ga1 Sm2 3.182(2) 1_565 ?
Ga1 Sm3 3.186(3) 2 ?
Ga1 Sm3 3.250(2) 7_556 ?
Ga1 Sm2 3.386(3) 8_566 ?
Ga2 Ga2 2.469(4) 7_556 ?
Ga2 Ga1 2.483(4) 2_665 ?
Ga2 Ga1 2.491(4) 3_565 ?
Ga2 Ga4 2.684(3) 2_665 ?
Ga2 Sm3 3.173(2) 3_665 ?
Ga2 Sm2 3.193(2) 3_665 ?
Ga2 Sm3 3.265(2) 9_666 ?
Ga2 Sm2 3.356(2) 9_666 ?
Ga3 Ga3 2.483(5) 9_556 ?
Ga3 Ga5 2.496(4) 8_566 ?
Ga3 Ga3 2.521(5) 8_676 ?
Ga3 Ga5 2.585(4) 3_565 ?
Ga3 Sm2 3.185(2) 8_566 ?
Ga3 Sm2 3.206(2) 1_565 ?
Ga3 Sm3 3.256(3) 7_556 ?
Ga3 Sm5 3.260(2) 7_566 ?
Ga3 Sm5 3.285(2) 1_565 ?
Ga3 Sm3 3.348(3) 2 ?
